Lithium vanadate Li~3+<i>x~</i>V~6~O~13~ at low temperature
Höwing, Jonas; Gustafsson, Torbjörn; Thomas, John O.; Acta Crystallographica Section C 60 (2004) i66–i68; doi:10.1107/S0108270104012508

data_2014094
_publ_section_title
;
 Lithium vanadate Li~3+<i>x~</i>V~6~O~13~ at low temperature
;
_journal_issue                   7
_journal_name_full               'Acta Crystallographica Section C'
_journal_page_first              i66
_journal_page_last               i68
_journal_paper_doi               10.1107/S0108270104012508
_journal_volume                  60
_journal_year                    2004
_chemical_formula_iupac          'Li3.24 V6 O13'
_chemical_formula_moiety         'Li3.24 V6 O13'
_chemical_formula_sum            'Li3.24 O13 V6'
_chemical_formula_weight         536.3
_chemical_name_common            'lithium hexavanadate'
_chemical_name_systematic        ' ?'
_space_group_IT_number           15
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 111.913(5)
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   21.487(5)
_cell_length_b                   3.9200(10)
_cell_length_c                   11.738(5)
_cell_measurement_reflns_used    1332
_cell_measurement_temperature    95
_cell_measurement_theta_max      100.737
_cell_measurement_theta_min      5.015
_cell_volume                     917.2(5)
_computing_cell_refinement       'SAINT-Plus (Bruker 2003)'
_computing_data_collection       'SMART (Bruker 2003)'
_computing_data_reduction        SAINT-Plus
_computing_molecular_graphics    'Diamond  (Berghoff, 1996)'
_computing_publication_material  Jana2000
_computing_structure_refinement  'Jana2000 (Petricek and Dusek, 2000)'
_computing_structure_solution    'program (reference)'
_diffrn_ambient_temperature      95
_diffrn_detector_area_resol_mean 512*512
_diffrn_measured_fraction_theta_full 0.95
_diffrn_measurement_device_type  'Bruker SMART APEX'
_diffrn_measurement_method       '\w scans'
_diffrn_radiation_monochromator  Si(111)
_diffrn_radiation_source         Synchrotron
_diffrn_radiation_type           Synchrotron
_diffrn_radiation_wavelength     0.872
_diffrn_reflns_av_R_equivalents  0.0428
_diffrn_reflns_av_sigmaI/netI    0.0536
_diffrn_reflns_limit_h_max       26
_diffrn_reflns_limit_h_min       -37
_diffrn_reflns_limit_k_max       6
_diffrn_reflns_limit_k_min       -4
_diffrn_reflns_limit_l_max       20
_diffrn_reflns_limit_l_min       -16
_diffrn_reflns_number            6862
_diffrn_reflns_theta_full        50.13
_diffrn_reflns_theta_max         50.52
_diffrn_reflns_theta_min         2.51
_diffrn_standards_interval_count 0
_diffrn_standards_number         0
_exptl_absorpt_coefficient_mu    10.337
_exptl_absorpt_correction_T_max  1.000
_exptl_absorpt_correction_T_min  1.000
_exptl_absorpt_correction_type   empirical
_exptl_absorpt_process_details   '(SADABS; Bruker, 2003)'
_exptl_crystal_colour            black
_exptl_crystal_density_diffrn    3.882(2)
_exptl_crystal_description       shard
_exptl_crystal_F_000             1007
_exptl_crystal_size_max          0.05
_exptl_crystal_size_mid          0.02
_exptl_crystal_size_min          0.01
_refine_diff_density_max         3.17
_refine_diff_density_min         -3.31
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   2.15
_refine_ls_number_parameters     102
_refine_ls_number_reflns         2499
_refine_ls_R_factor_all          0.0764
_refine_ls_R_factor_gt           0.0764
_refine_ls_shift/su_max          0.0094
_refine_ls_shift/su_mean         0.0003
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details     w=1/\s^2^(I)
_refine_ls_weighting_scheme      sigma
_refine_ls_wR_factor_gt          0.0687
_refine_ls_wR_factor_ref         0.0687
_reflns_number_gt                2499
_reflns_number_total             2500
_reflns_threshold_expression     I>-15\s(I)
_cod_data_source_file            bc1040.cif
_cod_data_source_block           I
_cod_original_cell_volume        917.3(5)
_cod_original_sg_symbol_H-M      'C 2/c'
_cod_database_code               2014094